2Test Result Relationships Importance of identifying trends.Help identify erroneous test results.Quality of pavementEncourage paying attention to test results.
3What is the end result we are looking for when involved in producing and placing an asphalt pavement? How do we as technicians effect the end result product?The end result is in the placement of a durable long lasting good quality asphalt pavement.Accurate test results, whether in the lab or field, are one important factor to achieving this.Pay factors are based on how well the QC techs do their job and also how well the QA tech does their job. Everything sampling, splitting and testing needs to representative of the mix being produced and placed. That means we need to be interested in everything that is going on the project, not just our stated job responsibity.Using test results that are not accurate will effect the quality of the HMA pavement and pay factors.
5Lab testing:RiceAC ContentsGradationsBulk Specific Gravities of coresField testing:Rice valueGauge SettingsTemperatures
6Production Mix design Production: Rice changes Gradation AC These changes can only be made after representative samples are acquired and properly tested.Accurate, comparable and repeatable test results, performed in an efficient manner and then communicated to the proper people.Such as Rice, unit weights, gradations….Techs are also of course involved in the aggregate testing and the mix design process.
7Where it StartsIt all begins with proper field sampling techniques and field sample sizes that are adequate. Next, the field sample must be split down to test size and still remain representative of the material being produced.How can accurate test results be acquired without a representative field sample? Adequate size for retesting, enough material so that you are not using outer edges, segregated areas, keep it mixedHow can accurate test results be acquired when a sample is improperly split and is not representative of the material sampled?
9What Effects What in the Lab? Rice value: Splitting, %AC & gradation, water temp, vibration, rodding.%AC: Splitting, gradation, % moisture, area around & in AC gauge, Correction Factors for Ignition Ovens.Gradations: Sampling, splitting, care in running the test.All effected by condition of testing equipmentScales level, screens clean, tears in screens, sagging screens, area around scales clean, flasks calibrated, check for chips in the lids or flasks, ignition oven clean including the venting, AC gauge clean, temperatures correct OVEN temps checked, sample temps checked
10What Effects What in the Field Percent Compaction: Rice value used, gauge settings, correction factors.Compaction: Temperature, roller pattern.Quality: Compaction
11Lab test results effect the roadway density, which effects the quality of the pavement. Lab test results are effected by the field sampling.
12Responsibility as materials technicians is the quality of the material that is produced and that it is placed properly.Even a good mix that meets all the mix design criteria, can still be poorly placed and have a disastrous end result.
13HMA Test Result Relationships Theoretical Maximum Specific Gravity or Unit Weight versus Roadway Density
14Rice & Density Summary of Test Relationships: Using a rice value that is too high will result in a calculated density that is actually lower than what the density of the roadway really is. This could result in over compaction of the mat.Using a rice that is too low will result in a calculated density that is actually higher than what the density of the roadway really is. This could result in under compaction of the mat
15Rice & DensityTheoretical Maximum Specific Gravity (rice) is the key measurement during both laboratory mix design and quality control procedures.Density can be calculated using Theoretical Maximum Specific Gravity commonly called the Rice Ex: 2.500Density can be calculated using Maximum Density (Unit Weight)/Wet Density which is the weight of a mix in pounds per cubic foot Ex pcfConverting back and forth is done by: Ex: X 62.4 = 156 pcf or156 / 62.4 =62.4 being the unit weight of waterEither method can be used to calculate a density.Using Maximum Density / Wet Density of the mix is now the more common method when using M/D nuclear gauges out in the field performing mat densities.Specific gravity = equal volume of water & a stated temperature.
16About HMA DensityPavement is to be compacted to 94% +/- 2% density to achieve a durable pavement. That is 94% +/- 2% of the Theoretical Maximum Specific Gravity (rice) or maximum density (pcf) of the mixture.Accurate, repeatable, comparable results done in a timely manner and then communicated to the proper people.
17Rice & DensityWe are looking for 8% air voids (92% compaction) to 4% air voids (96% compaction) and preferably 6% air voids (94% compaction) in the completed mat.A certain percent of air voids are necessary in the finished HMA.
18Rice & DensityRice or maximum density not representative of the mix being placed:Causes either an over or under-compacted mat.Calculated percent compaction becomes just a number that is not accurate or a true reflection of the density of the mat.What happens to the pavement quality.Over compaction can lead to rutting, flushing or bleeding, resulting in a shortened pavement life and even dangerous driving conditions.Under compaction can lead to pavement susceptibility to moisture and air damage, shortening the life & durability of the asphalt pavement.
20Nuclear GaugeCheck the settings in your gauge MA for asphalt.Correct maximum density in-put into the gauge.Using the correct Correction Factors?Correction Factors correlate gauges to mat for accurate compaction.Gauge clean and flush with the pavement. Record CF on test report, so that it can be verified that the correct CF is being used.
21HMA Test Result Relationships Rice ver. Asphalt Content
22Rice ver. Asphalt Content Summary of Test Relationships:As the asphalt content increases, the rice value will decrease.As the asphalt content decreases, the rice value will increase.
23Rice ver. AC ContentThe aggregate must be coated with the percent binder as per determined in the mix design.Too much binder, unstable mat resulting in ruttingToo little binder, uncoated aggregate – open to moisture susceptible & stripping or a dry mix that does not compact well and is unstable.Amount of binder effects the rice value:Inconsistent compaction.Effects quality of pavement.
24Talk about mix design ver plant produced…changing the rice to representative of the mix being placed.Formula in CP-56* May be that the sp g of the agg has changed, which in turn means new VMA..has to meet min requirements that are specified..if don’t, new mix design. Work suspended.
25Rice ver AC ContentThe Rice value changed with the plant produced material.Adjust the rice for field produced material, so that the rice value being used is correct for accurate % compaction.Ex: Field Sp G of / (Form 43)= 94.9%Field Sp G of / (New Target Rice) = 95.9%Difference of 1%% CompactionCP-56 info ac contents, effective sp g of agg,Mix 4% voids…comp. to 8-4% voids …?Once AGAIN, SEE HOW TEST EFFECTS TEST..AC’S, HAS THE BULK SP G’S OF AGG CHANGED???
26Change in the Bulk Specific Gravity of the Aggregate. New Rice = New VMA, that still has to meet the minimum requirements.VMA – what is itNew Mix design
27AC Content & RiceDoes the GRADATION of a sample affect the results for AC or Rice?Effects AC content.Effects Rice results.
28How does Gradation Affect Test Results? Coarse sample will result in a lower AC content.Fine sample will result in a higher AC content.Remember the trend of AC ver Rice.Due to sampling or splitting?A too coarse or too fine gradation will also affect the rice results. If the gradation is unrepresentative, then the rice result on that sample is not going to be correct to be used on the roadway!
29Use a representative rice value to ensure that proper compaction takes place on the roadway and that no densities are failing or passing as the result of using rice values that are not representative of the mix being placed.It is a good practice to always have a copy of the mix design handy and check what the rice value should be for that that % AC whether you are a lab tech or the field tech.Also, have a copy of the daily average rice values along with the AC contents of each rice, if on a CDOT project. Try to pay attention to the relationships.
30HMA Test Result Relationships What affects a Rice Value?
31What Effects a Rice Value… Temperatures, aggregate absorption, cure times, sampling, splitting, testing equipment.Rice values change as the asphalt absorbed into the aggregate varies with a given mixtureCure times-The amount of asphalt absorbed into the aggregates during production, placement and compaction of the mixture will be a function of several factors. Plant mixing temperatures, absorption characteristics of the individual aggregates and the blend itself, and the amount of time the mixture is maintained at elevated temperatures.- The weight of materials remains constant, because the total asphalt content remains constant, but it is the overall volume of the mixture that decreases as asphalt is absorbed into the aggregate.A mix design is based on a volume basis.
32Cure Times of the MixStandard practice for cure times or aging periods, is at compaction temperature, minus anytime sample has already had to age or cure.A sample of mix taken at the plant, and immediately taken to the lab for testing, needs to be aged before the rice testing begins. (CDOT – temp above 200’ F)
33Cure Times Field samples have aged by the time they reach the lab. As per CDOT, if a sample cannot be tested & compacted in the agreed upon conditioning time, it should be allowed to cool and reheated.Samples should never be kept at compaction temperature longer than 4 hours.
34Each sample should be vibrated and rodded the same through out production. One other important item that needs to be mentioned, is the water for the test sample needs to be the same temperature used when calibrating the flask or adjusted.Method of vibration, mechanical, by hand…rod or not rod…
35HMA Test Result Relationships Air Voids versus Gradation
36Air Voids versus Gradations The durability of an asphalt pavement is a function of the air void content.Air voids = compaction = durabibilityAggregate gradation is what makes the strong stone skeleton to enhance resistance to permanent deformation and allows for sufficient void space to enhance mixture durability.Discuss this to know the importance of having enough air voids and not to high of air voids in the mix.
37HMA Test Result Relationships High Asphalt Content ver. Low Asphalt Content
38High ver. Low Asphalt Content Test result relationships:Low asphalt content = high air voidsLow asphalt content = higher maximum specific gravity (rice)High asphalt content = low air voidsHigh asphalt content = lower maximum specific gravity (rice)
39How the quality of HMA is affected by low asphalt contents because of a higher percentage of air voids:Susceptible to dryness or ravelingImpermeability is decreased - causing susceptible to moisture damage and strippingThin film coating on the aggregate which can increase the speed at which oxidation takes place, causing early aging and loss of roadway life.Low asphalt content can lead to fatigue cracking. Fatigue cracking is a result of the pavements lack of resistance to repeated bending under wheel loads (traffic).Whether by design or lack of compaction, fatigue resistance is also drastically reduced by high percentage of air voids which can be caused from low asphalt content.Flexibility of an asphalt pavement is affected by low asphalt content (fatigue cracking)Maximizing the asphalt film thickness increases durability, so low asphalt content will decrease the durability.
40How the quality of HMA is affected by high asphalt contents because of a lower percentage of air voids:Pavement can become unstable at a high asphalt content resulting in rutting, wash boarding, flushing or bleeding.Bleeding can cause low skid resistance.The higher the asphalt content , the lower the air voids.Increases the VFA (voids filled with asphalt) and takes the space for air voids.VMA (voids in the mineral aggregate) will generally decrease slightly to a minimum value then increase with increasing asphalt contents becoming unstable.Unit weight (density) of the total mix generally rises with increased asphalt content and then falls and becomes unstable, low air voids.
41HMA Test Result Relationships The Importance of Temperatures and Compaction
42Temperatures & Compaction Even a good mix, if not compacted properly will not result in a long lasting durable asphalt pavement .The lab testing will show what the mix is capable of in it’s performance, but the actual compaction process will determine the life and durability of the roadway.Proper temperatures during the compaction.Asphalt binder is a thermoplastic, temperature susceptible material.
43Temperatures & Compaction As binder cools it becomes stiffer and bonds the aggregates to provide a durable structure.Compaction needs to be complete before the mixture temperature falls below the recommended range for the type of PG binder being used.Continuing to compact can damage the pavement.
44Temperatures & Compaction The temperature of a mixture is perhaps the most important property in obtaining density, since the viscosity of an asphalt binder is controlled by its temperature.Obtaining density is perhaps the most important process for a durable long lasting asphalt pavement.
45What all is involved in obtaining density? Field sampling - representativeSplitting to test size - representativeLab tests for AC, gradation, rice value – accurate, representative – Quality ControlGauge settings – max. density, corr. factors - accurateCompaction – temperatures, rice valuesQuality pavement